# Semiconductor Devices

Embed Size (px)

### Transcript of Semiconductor Devices

- 1 -1/15/02C:\lec320.doc

H.L.Kwok

SEMICONDUCTOR MATERIALS AND DEVICESby H.L. Kwok

Objective: The purpose of these notes is to familiarize students with semiconductors and devices including the P-N junction, and the transistors.

1

1

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

Part 1: Semiconductor Materials

What we need to learn. a. Semiconductor structures b. Electronic properties c. Intrinsic and extrinsic semiconductors

Part 1: Semiconductor Materials

2

2

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 3 -1/15/02C:\lec320.doc

H.L.Kwok

A.

Properties

Semiconductors occupy a small fraction of the Periodic Table. The word semiconductor means a material having conduction properties half-way between a conductor and an insulator.

3

3

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

Solids are often classified according to their conductivity and semiconductors have conductivities in the range of 10 4 - 10-6 S/m. Fig.1.1 shows the conductivity range of semiconductors. Semiconductors that are of interest to us include: silicon (Si), germanium (Ge) and gallium arsenide (GaAs).

a) Crystal structures Si and Ge have the diamond crystal structure.

The diamond crystal structure is formed by 2 interlaced fcc unit cells. The cells are displaced by 1/4 the distance along the body diagonal. Fig.1.2 shows the diamond crystal structure. GaAs has the zinc-blende crystal structure (similar to the diamond structure except that the Ga atoms and the As atoms occupy different lattice sites). This is illustrated in Fig.1.3.

In these crystals, the bonding arrangement between the nearest neighbors is tetrahedral (i.e., each atom has 4 nearest neighbors). The bond angle is shown in Fig.1.4. Semiconductors have covalent bonds. For covalent bonds, the electrons are shared between the nearest neighboring atoms as shown in Fig.1.5.

Example 1.1: At 300K, the lattice constant for Si is 0.543 nm, calculate the number of Si atoms/m3.44

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 5 -1/15/02C:\lec320.doc

H.L.Kwok

Solution: Each unit cell of the fcc structure has 4 atoms. Therefore, the diamond structure has 8 atoms per unit cell. The volume of the unit cell V = (5.43 x 10 -10)3 m3 = 1.6 x 10-28 m3. The number of atoms per unit volume N = 8/(1.6 x 10-28) /m3 = 5 x 1028 /m3. #

Lattice direction is a vector represented by the symbol: [x y z], where x, y, and z are the values of the lattice coordinates (of the vector) measured from the origin (a chosen lattice point). Lattice directions parallel to one another belong to the same family and are represented by the same symbol (in angular brackets). A lattice plane is represented by a set of numbers (h k l) known as the Miller indices. h, k, and l are the normalized values of the inverse of the interceptions of the plane on each of the coordinates.

Example 1.2: A lattice plane intercepts the principal axes at positions: a, 2a, 2a. Determine the Miller indices. Solution: The Miller indices are: (211). This is illustrated in Fig.1.6. #

5

5

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

B.

Electronic properties of semiconductors

A semiconductor at low temperature is similar to an insulator and the energy bonds are intact. There are very few free electrons at low temperature.

As temperature increases, some energy bonds are broken and the density of electrons increases. The density of electrons is quite small (~ 1012-19 /m3) at room temperature.

Creation of free electrons is accompanied by the creation of holes. A hole is a broken energy bond with a missing electron. Holes are positively charged and their motion also leads to current flow. A hole moves when the hole is filled with an electron. This is illustrated in Fig.1.7.

For an intrinsic semiconductor, the electron density n equals to the hole density p, i.e., n = p.

Example 1.3: Intrinsic Si has 1.45 x 1016 /m3 of electrons and holes, respectively. If n = 0.15 m2/V.s and p = 0.045 m2/V.s, determine the conductivity.66

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 7 -1/15/02C:\lec320.doc

H.L.Kwok

Solution: The conductivity = nqn + pqp = 1.45 x 1016 /m3 x 1.6 x 10-19 C x (0.15 + 0.045) m2/V.s = 0.45 x 10-3 S/m. # (Remember we mentioned earlier on that for a semiconductor lies between 104 to 10-6 S/m.)

a)

Energy bands

Electrons and holes in a semiconductor are allowed to possess specific energy ranges. These energy ranges are called energy bands. Traditionally, engineers are interested in electrons and energy bands are constructed with electrons in mind, i.e., they are plotted in terms of negative potential energy. Thus, in a typical energy band diagram, electron energy (negative potential energy) is plotted upward, while hole energy (positive potential energy) is plotted downward. Fig.1.8 shows the energy band diagram for Si. Crystal momenta (along two different crystal directions) are plotted along the horizontal axes. The symbol E stands for electron energy.

Since electrons normally reside in the lowest energy states in a solid, electrons will first fill up the lower energy bands. When these are filled, they start to fill the higher energy bands. As a

7

7

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

result, some higher energy bands will be partly filled. These are called conduction bands. They are illustrated in Fig.9.

Partially emptied energy bands have holes and they are called valence bands.

The energy difference between the conduction band edge and the valence band edge is the energy gap. Electrons and holes are not allowed to have energies falling within the energy gap. Effectively, energy gap is the amount of energy needed to form an electron and a hole.

The shape of an energy band changes with temperature, pressure, etc. For instance: the energy gap Eg(T) of Si has the following temperature dependence: Eg (T) = 1.17eV - 4.73 x 10-4 T2/(T + 636 K) eV where T is the absolute temperature. This dependence is shown in Fig.1-10. (1-1)

Example 1.4: What is Eg for Si at 300 K? Solution:

8

8

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 9 -1/15/02C:\lec320.doc

H.L.Kwok

From Eqn.(1-1): Eg (T = 300 K) = 1.17 - 4.73 x 10 -4 x 3002/(300 K + 636 K) eV = 1.12 eV. #

b)

Electron motion

Motion of electrons and holes is affected by the lattice potential. This may be viewed as an interaction between the electron/hole and the lattice vibrations. The result is that electrons and holes appear to possess masses different from the electron rest mass, m0.

These are called effective masses, (me* for electrons, and mh* for the holes) and they are less than m0. The small masses imply that the lattice vibrations appear to assist in the motion of the electrons and the holes. For Si at 300 K: me* (electrons) = 0.33 m0, and mh* (holes) = 0.55 m 0.

c)

Density of states for the electrons and holes An energy band contains many energy levels/states.

Electrons occupying energy levels/states obey the Pauli exclusion principle - which states that there can be at most 2 electrons per energy state.99

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

The density of states in an energy band is given by the density of states function S(E) given by: S(E) = 4 [2mb*/h2]3/2E1/2 (1-2)

where mb* is a density of states mass parameter and h (= 0.662 x 1033 J.s) is the Plancks constant. S(E) has the dimension of per unit volume per unit energy.

To compute the electron density n, S(E) is multiplied to a probability function that characterizes the occupation of the different energy states. This probability function is the FermiDirac function f(E). f(E) = 1/[1 + exp((E - EF)/kT)] (1-3)

where EF is the Fermi-level, E is the energy of the electron, k (= 1.38 x 10-23 J/K) is the Boltzmann constant, and T is the absolute temperature.

Based on the above, the electron density n in the conduction band is given by: n = Ec Se(E)/[1 + exp((E - EF)/kT)].dE (1-4)

where Se is the density of states in the conduction band, E F is the Fermi-level, and EC is the energy at the conduction band edge. A graphical plot of Se and f(E) versus E is shown in Fig.1-11.1010

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 11 -1/15/02C:\lec320.doc

H.L.Kwok

A similar expression for the hole density p in the valence band is given by: p = - Ev Sh(E)/[1 - exp((E - EF)/kT)].dE (1-5)

where Sh(E) is the density of states in the valence band, and E V is the energy at the valence band edge.

If we assume that both |EC - EF| and |Ev - EF| >> kT, n NC exp[- (EC - EF)/kT] p NV exp[- (EF - Ev)/kT] (1-6)

where NC (= 2 x (2 mb*kT/h2)3/2) is the effective density of states in the conduction band, and NV (= 2 x (2 mb*kT/h2)3/2) is the effective density of states in the valence band. At 300 K, NC = 2.8 x 1025 /m3 and NV = 1.04 x 1025 /m3 for Si.

According to Eqn.(1-6), electron and hole densities depend on the position of the Fermi-level. This is illustrated in Fig.1-12.

Example 1.5: Compute the electron density in Si if the Fermi level is at 0.55 eV below the conduction band edge. Assume T = 300 K (kT at 300 K = 0.0259 eV). Solution:

11

11

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

From Eqn.(1-5): The electron density n = NC exp(- (EC - EF)/kT) = 2.8 x 1025 /m3 x exp(- 0.55 eV /0.259 eV) = 1.67 x 10 16 /m3. #

d)

Intrinsic semiconductor An intrinsic semiconductor is one with no impurities.

For an intrinsic semiconductor, n = p = n i, the intrinsic carrier density.

Using Eqn.(1-6), the intrinsic carrier density is given by: ni = [NC NV exp(- Eg/kT)]1/2 where we have substituted Eg = EC - EV. (1-7)

At 300 K, ni = 1.45 x 1016 /m3 for Si.

Note that: pn = ni2.

This is a very important relationship and is a consequence of the law of mass action - which states that the product of the electron density and the hole density is a constant at a given temperature.

For an intrinsic semiconductor, we have E = E i, the Intrinsic Fermi- level.

12

12

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 13 -1/15/02C:\lec320.doc

H.L.Kwok

It can be shown that: Ei = Eg/2 + kT/2 ln(NV/NC) When NV = NC, Ei is at the middle of the energy gap. (1-8)

e)

Extrinsic semiconductors

Semiconductors become extrinsic when impurities are added. This is achieved with the addition of donors or acceptors. Impurities are called donors/acceptors depending on whether electrons/holes are produced.

Structurally, donors are similar to the semiconductor (host) atoms except that there are 5 electrons in the outermost orbits (versus 4 electrons for the (host) semiconductor). Ionization of the donor atom generates an electron. Acceptor atoms have 3 electrons in the outermost orbits and the capture of an electron from a neighboring atom will generate a hole in the neighboring atom. This is illustrated in Fig.1-13.

Because of their low ionization energies, donors and acceptors are fully ionized at room temperature. This results in: n = ND or, p = NA, where ND is the donor density and NA is the acceptor density.1313

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

A semiconductors is N-type when n >> p, and P-type when p >> n.

In the presence of donors/acceptors, electron and hole densities will change. Since the law of mass action dictates that pn = n i2, p = ni2/ND for a N-type semiconductor and n = ni2/NA for a P-type semiconductor.

For an extrinsic semiconductor, the position of the Fermilevel moves away from the intrinsic position. For an N-type semiconductor (n = ND), EC - EF = kT ln(NC/ND) Similarly, for a P-type semiconductor (p =N A), EV - EF = - kT ln(NV/NA) (1-9)

Fig.1-14 shows the positions of the Fermi-levels in an N-type semiconductor and in a P-type semiconductor, respectively.

If both donors and acceptors are present in a semiconductor, the dopant in greater concentration dominates, and the one in smaller concentration becomes negligible. Semiconductors are named after the dominant carrier type.1414

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 15 -1/15/02C:\lec320.doc

H.L.Kwok

Thus, an N-type semiconductor has more electrons than holes, while a P-type semiconductor has more holes than electrons. The dominant carrier is called the majority carrier versus the term minority carrier for the carrier in lesser quantity.

It is sometimes more convenient to express n and p in terms of the intrinsic Fermi-level E i, i.e., n = NC exp(- (EC - EF)/kT) = NC exp(- (EC - Ei)/kT) exp(- (EF - Ei)/kT) = ni exp((EF - Ei)/kT) (1-10)

Similarly, p = ni exp((Ei - EF)/kT) (1-11)

Using this representation, one reduces the number of unknown parameters for the above equations of n and p from 3 (NC, NV, EC/EV) to 2 (Ei and ni).

Example 1.6: Find EC - EF if ND = 1 x 1022 /m3 for Si at 300 K. Solution: From Eqn.(1-10), EC - EF = kT ln(NC/ND) = 0.0259 eV x ln(2.8 x 1025 /m3/1 x 1022 /m3) = 0.2 eV. #

15

15

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

Example 1.7: If Si is doped with 1 x 1020 donors/m3, compute the carrier densities at 300 K. Solution: From Eqn.(1-8): n = ND = 1 x 1020 /m3 and p = ni2/ND = (1.45 x 1016)2/(1 x 1020 /m3) = 2.1 x 1012 /m3. #

f)

Dopant energy levels

Table 1.1 shows the dopant ionization energies in common semiconductors at 300 K:Phosphorus Si Ge GaAs 0.045 0.012 0.026 Arsenic 0.049 0.0127 Boron 0.045 0.0104 -

Table 1.1: Dopant ionization energies in the common semiconductors (measured in eV from the band edges: i.e., NC in the case of the donors and NV in the case of the acceptors).

The ionization energies may be compared to the thermal energy kT (= 0.0259 eV) at 300 K. Fig.1-15 shows the positions of dopant energy levels in an energy band diagram.

g)

Temperature dependence of the carrier densities1616

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 17 -1/15/02C:\lec320.doc

H.L.Kwok

Electron and hole densities in an extrinsic semiconductor can vary with temperature. At a low temperature, not all of the dopant is ionized and the majority carrier density will be small. Nevertheless, its density is still much larger than the intrinsic carrier density. At high temperature, the intrinsic carrier density increases rapidly, while ND or NA remains unchanged. At a sufficiently high temperature, the semiconductor becomes intrinsic. The variation of the electron density n versus the inverse temperature in an N-type semiconductor is shown in Fig.1-16.

17

17

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

Part 2: Carrier transport

What we need to learn. a. b. c. d. e. Electronic motion Conduction properties of electrons and holes Drift and diffusion Generation and recombination Continuity equations

18

18

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 19 -1/15/02C:\lec320.doc

H.L.Kwok

Part 2: Carrier transport Carrier transport refers to the movement of the electrons and holes in a semiconductor under an applied voltage. The simplest types of carrier transport are by drift and diffusion. Drift is charge flow as a consequence of the presence of an applied electric field, while diffusion is charge flow due to the presence of a carrier density gradient.

A.

Random motion of the electrons

At room temperature, electrons possess thermal energy and its value is 3kT/2. Equating this thermal energy to the kinetic energy of an electron will give: me*vth2/2 = 3kT/2 (2-1)

where me* is the effective mass of the electron, and v th is the thermal velocity.

It can be shown that at T = 300 K, the thermal velocity v th 1 x 105 m/s. This suggests that electrons in a semiconductor are moving at a very high speed.

19

19

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

B.

Electrons in an electric field

An electric field E imposes a preferred direction of motion for the electrons. This is superimposed on top of the random motion. Because of their charge, electrons will move in opposite direction to the applied electric field (holes actually move in the same direction) The motion of the electrons and the holes will stop when they encounter collisions. This is illustrated in Fig.2.1.

Assuming a mean free time c between collisions for the electrons, Newtons law gives: - qE = me* vd/c where vd is the drift velocity of the electrons. This leads to: vd = - qcE/me* (2-3) (2-2)

By definition: the electron mobility n = - vd/E. We have: n = qc/mn* Note that: n is positive. (2-4)

20

20

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 21 -1/15/02C:\lec320.doc

H.L.Kwok

Collision of a hole can be viewed as an interruption in the filling of the hole by an electron. The drift velocity is then given by: vd = qc* E/mh* (2-5)

where c is the mean free time of the holes, and mh* is the hole effective mass. This leads to: p = qc* E/mh* (2-6)

According to Eqns.(2-5) and (2-6), the mean free times of the electrons and the holes determine their mobilities.

Collision is also referred to as scattering. Theoretically, it can be shown that: c ~ T-3/2 for lattice scattering, and c ~ T3/2 for ionized impurity scattering.

When more than one type of scattering is present, the shortest mean free time dominates. This also applies to the carrier mobility since mobility is directly proportional to the mean free time.

In general, the combined mobility T in the presence of more than one type of scattering is given by: T-1 = i I-1 (2-7)

21

21

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

where i is the mobility due to the ith scattering. The process is shown in Fig.2.2. From the carrier mobility, one can compute the drift velocity.

Example 2.1: At 300 K, n = 0.15 m2/V.s. Determine its value at 200 K if lattice scattering dominates. Solution: n(T = 200 K) = n(T = 300 K) (300 K/200 K)3/2 = 0.15 m2/V.s x 1.84 = 0.275 m2/V.s. #

Current density is the charge flow through a unit area cross-section in unit time. Consider a unit volume in a semiconductor, the amount of electrons Q inside this unit volume is given by: Q = - nq, where n is the electron density, and q is the electron charge. If this quantity of charge Q moves through a distance x in time t, the electron current density Jn (= Q x/t = Qvd) is given by: Jn = - qnvd Similarly, hole current density J p = qpvd. (2-8)

The total current density JT is given by: JT = Jn + Jp = - qnvd + pqvd22

(2-9)22

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 23 -1/15/02C:\lec320.doc

H.L.Kwok

Since n = - vd /E and p = vd/E, JT = (nqn + pqp) E = E where is the conductivity of the semiconductor. Note that the inverse to conductivity is the resistivity. (2-10)

For a measurement of resistivity, a 4-point probe method is frequently used. The measurement setup is shown in Fig.2.3. In the measurement, a current is supplied to the semiconductor wafer through the outer probes and a voltage is measured across the inner probes. For a thin sample, resistivity is given by: = V/I x 4.54 t .m (2-11)

where V is the measured voltage, I is the current through the outer probes, and t is the thickness of the wafer. Note that the probe separation has been assumed to be small compared to the other dimensions.

Example 2.2: If p = 0.045 m2/V.s at 300 K, compute the drift velocity when E = 100 V/m. Solution: From Eqn.(2-5), vd = p E = 0.045 m2/V.s x 100 V/m = 4.5 m/s. #

23

23

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

Example 2.3: In a 4-point probe measurement, if V = 1 V and I = 1 mA, determine if t = 200 m. Solution: From Eqn.(2-11), = V /I x 4.54 t .m = 1 V/1 x 10-3 A x 4.54 x 200 x 10-6 m = 0.91 .m. #

C.

Diffusion current

Diffusion of carriers occurs in the presence of a carrier density gradient. For electrons, the rate of electron flow per unit area n in 1dimension is given by: n = - Dn dn/dx where Dn is the electron diffusivity. (2-12)

Electron diffusion current density is then given by: Jn = - qn = qDn dn/dx Similarly, hole diffusion current density is given by: Jp = - qDp dp/dx where Dp is the hole diffusivity. (2-14) (2-13)

24

24

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 25 -1/15/02C:\lec320.doc

H.L.Kwok

Fig.2.4 shows the relationship between the diffusion currents and the carrier density gradients.

Sometimes, diffusivity is expressed in terms of a mean free path for the carrier. For electrons, we can write: Dn = vth, where vth is the thermal velocity. The mean free path may be expressed in terms of the collision time, i.e., = vthc.

a)

Einstein relation

In 1-dimension, for a collection of electrons we have: m e* vth2 /2 = kT/2, and Dn = vth = vth2c = kT c/me*. Since n = qc/me*, Dn = n kT/q (2-15)

This equation is known as Einstein relation. Einstein relation allows one to relate Dn to n. A similar expression exists for the holes.

Example 2.4: If n = 0.15 m2/V.s at 300 K for a semiconductor, compute D n. Solution: From Eqn.(2-15): Dn = n kT/q = 0.15 m2/V.s x 0.0259 V = 3.89 x 10-3 m2/s. #2525

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

b)

Drift and diffusion current densities

Currents for electrons and holes are due to drift and diffusion. In 1-dimension, the electron and hole current densities are given by: Jn = qnn E + qDn dn/dx Jp = qpp E - qDp dp/dx (2-16)

The total current density JT is given by: JT = J n + J p (2-17)

D.

Carrier injection

In thermal equilibrium, we have pn = n i2. Carrier injection in a semiconductor results in: pn > n i2.

Assuming that the equilibrium carrier densities are given by: n0 and p0, we can define the excess carrier densities as: n = n - n0, and p = p - p0. The extent of charge injection depends on the amount of excess carriers.

26

26

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 27 -1/15/02C:\lec320.doc

H.L.Kwok

High-injection implies that: n >> n0 and p >> p, while lowinjection implies either n >> n0 and p p0 (in an N-type semiconductor).

Example 2.5: If n0 = ND = 1 x 1022 /m3 for a N-type Si sample, and n = p = 1 x 1015 /m3, what type of injection occurs. Solution: This will be low-injection as: p 0 = ni2/ND = (1.45 x 1016 /m3)2/1 x 1022 /m3 (p0 > Gth) and G = p/p. This leads to (for low-injection): p = p0 + Gp (2-20)

b) Dynamic response The dynamic change of hole density in a semiconductor is given by: dp/dt = G - R (2-21)

In the absence of external generation, G = Gth, we have: dp/dt = U = (p - p0)/p. This leads to: p = p0 + Gp exp(- t/p ) (2-22)

where we assumed that the initial hole density is: p 0 + Gp.

29

29

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

The hole density (= (p0 + Gp) at t = 0) relaxes exponentially towards it equilibrium value p 0. This is illustrated in Fig.2-6.

Example 2.7: At t = 0-, G = 1 x 1024 /m3.s. Determine the hole density in a semiconductor at t = 1 ms if G = 0 when t > 0. Neglect the value of p0 and assume p = 0.1 ms. Solution: Based on Eqn.(2-22): p = p0 + Gp exp(- t/p ) = 1 x 10-4 s x 1 x 1024 /m3.s exp(- 1 x 10-3 s/1 x 10-4 s) = 4.54 x 1015 /m3. #

c) Indirect recombination Indirect recombination occurs at impurity centers with energy level(s) in the energy gap.

When compared with band-to-band recombination, such as a process is favored because it involves smaller energy transitions. Fig.2.7 shows a schematic of the recombination of an electron and a hole via an impurity center. The lifetime of electrons/holes varies with the density of the impurity center. To first order, the lifetime of carriers is inversely proportional to the impurity density NI.

30

30

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 31 -1/15/02C:\lec320.doc

H.L.Kwok

d)

Continuity equation

The 1-dimensional continuity equations for electrons and holes include drift, diffusion, generation and recombination. They are given by: dn/dt = (1/q) dJn/dx + (Gn - Rn) dp/dt = - (1/q) dJp/dx + (Gp - Rp) (2-23)

The subscripts p and n denote the electron and hole contributions.

In full, these equations can be written as (for the minority carriers only): dnp/dt = npn dE/dx + nE dnp/dx + Dnd2 np/dx2 + Gn - (np - np0)/n dpn/dt = - pnpdE/dx - pE dpn/dx + Dpd2 pn/dx2 + Gp - (pn - pn0)/p (2-24) The product (Dpp) (= Lp) is the hole diffusion length. Similarly, the electron diffusion length is given by: Ln = (Dnn).

Example 2.8: Write down the steady-state continuity equation for hole minority carriers when E = 0 and Gp = 0. Assume pn = pno when x = . Solution:

31

31

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

From Eqn.(24): in the steady state: dpn/dt = - pnp dE/dx - pE dpn/dx + Dp d2 pn/dx2 + Gp - (pn - pn0)/p = 0. Since E = 0 and Gp = 0, only the last term remains, i.e., Dp d2 pn/dx2 = (pn pn0)/p. The solution to this equation will be: pn = pn0 + (pn(0) - pn0) exp(x/(Dpp)), where pn(0) is the hole density when x = 0.

Example 2.9: Light is allowed to fall on 1 side of a semiconductor sample and pn(0) = 1 x 1022 /m3. If p = 100 s and Dp = 1 x 10-3 m2/s, determine pn when x = 1 mm. Assume pn0 = 1 x 1011 /m3. Solution: From the previous example: pn = pn0 + (pn (0) - pn0)exp(- x/(Dpp) = 1 x 1011 /m3 + (1 x 1022 /m3 - 1 x 1011 /m3) x exp( - 1 x 10-3 /m/(1 x 10-4 m2/s x 1 x 10-3 s) = 4.2 x 1020 /m3. #

Example 2.10: Assume pn = pn0 at x = w, determine the hole current density based on the conditions specified in Example 2.9. Assume w > Lp, it can be shown that: Jp = q(pn (0) pn0)Dp/w. Note in this example that the approximation w > ND, we have: W xn = [2s Vbi/(qND)] E = - qNDW(1 + x/W)/s = Vbi(- 2x x2/W)/W39

(3-13)39

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

Example 3.2: For a 1-sided step junction with NA = 1 x 1025 /m3 and ND = 1 x1021 /m3, compute the value of W and E m at T = 300 K. Solution: From Eqn.(3-5), Vbi = (kT/q) ln(NAND/ni2) = 0.0259 V x ln(1025 X 1021/(2.1 x 1032) = 0.874 V. From Eqn.(3-13), W xn = (2s Vbi/(qND)) = 3.37 x 10-7 m. qNDW/s = - 5.4 MV/m. # Em = -

c)

Depletion capacitance

The donor and acceptor charge layers in the P-N junction give rise to the depletion/junction capacitance. This is illustrated in Fig.3.11

The depletion capacitance per unit area Cj is given by: Cj = dQ/dVa = s/W where Q is the charge density per unit area. (3-14)

For a 1-sided step junction: Cj = [qsNB/(2(Vbi - Va))]1/240

(3-15)40

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 41 -1/15/02C:\lec320.doc

H.L.Kwok

Fig.3.12 shows a typical plot of 1/C2 versus Va.

Example 3.4: An abrupt P-N junction has a doping concentration of 1021 /m3 on the lightly doped N-side and of 1025 /m3 on the heavily doped Pside. From a plot of 1/C2 versus Va, comment on values of the slope and the intercept on the voltage axis. Solution: NB = ND = 1021 /m3. The governing equation (Eqn.(3-15)) is 1/C2 = 2(Vbi Va)/(qsNB). Such a plot will give a straight line with a negative slope and the interception on the voltage axis is V bi. #

B.

I-V characteristics

I-V characteristics of a P-N junction behave differently under forward bias versus reverse bias.

Ideal I-V characteristics are obtained under the following assumptions: Abrupt junction

Carrier densities at the junction boundaries are directly related to the electrostatic potential Low-injection

No generation and recombination current in the depletion region

41

41

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

With bias, the electron density in the N-side at equilibrium is given by (see Eqn.(1-10)): nn0 = ni exp((EF - Ein)/kT) where Ein is the intrinsic Fermi-level on the N-side. (3-16)

On the P-side, one has: np0 = ni exp((EF - Eip)/kT) where Eip is the intrinsic Fermi level on the P-side. The subscript 0 stands for the case of equilibrium. (3-17)

Since Eip - Ein = qVbi, we have: nn0 = np0 exp(qVbi/kT) (3-18)

For an applied voltage equal to Va, the Fermi-level will split up as shown in Fig.3.13.

Electron density at the edge of the depletion region depends exponentially on the built-in voltage. We can now replace Vbi by Vbi - Va; nn0 by nn; and np0 by np in our equations.

42

42

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 43 -1/15/02C:\lec320.doc

H.L.Kwok

This leads to: nn = np exp(q(Vbi - Va)/kT) (3-19)

At low-injection, nn = nn0 and we can equate Eqns.(3-18) and (319). This leads to: np = np0 exp(qVa/kT) (3-20)

From Eqn.(3-20), we see that across the P-N junction, the minority carrier density is increased by exp(qV a/kT). A similar situation exists in the N-side and we have: pn = pn0 exp(qVa/kT) (3-21)

To determine the diffusion currents, we combine Eqns.(3-20), (321) and the continuity equation. This gives: Dn d2np/dx2 - (np - np0)/n = 0 Dp d2pn/dx2 - (pn - pn0)/p = 0 The boundary conditions are: x = y = 0: pn = pn0 exp(qVa/kT); and np = np0 exp(qVa/kT) x = y = : pn = pn0; and np = np0 They result in: pn - pn0 = pn0 [exp(qVa/kT) - 1] exp(- x/Lp)4343

(3.22)

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

np - np0 = np0 [exp(qVa/kT) - 1] exp(- y/Ln) These excess carrier densities are plotted in Fig.3.14.

(3-23)

The above equations also lead to: Jp = - qDp dpn/dx = qDppno/Lp [exp(qVa/kT) - 1] Jn = qDn dnp/dx = qDnnpo/Ln [exp(qVa/kT) - 1] (3-24)

where Jn and Jp are the electron and hole current densities, respectively.

The total current density JT is: JT = Jn + Jp = Js [exp(qVa/kT) - 1] where Js = qDppno/Lp + qDnnpo/Ln. This is called the ideal diode equation and the I-V characteristics are shown in Fig.3.15. (3-25)

Example 3.5: An ideal P-N junction has N D = 1024 /m3 and NA = 10 22 /m3, p = n = 1 s and a device area of 1.2 x 10-9 m2, calculate the ideal saturation current at 300 K. (It can be shown that: D p = 0.00116 m2/s and Dn = 0.00388 m2/s.) Solution: For an ideal device, the recombination current is assumed to be zero.

44

44

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 45 -1/15/02C:\lec320.doc

H.L.Kwok

From Eqn.(3-24), we can out it into the form: I s = Js x Acs = (qDpni2/(LpND) + qDnni2/(LnNA)) x Acs = (q x ni2 x Acs) x ((Dp/p)0.5 ND + (Dn/n)0.5NA) = (1.6 x 1019 C x 2.1 x 1032 /m6 x 1.2 x 10-9 m2) x ((0.00116 m2/s/10-6 s)0.5/1024 /m3) + ((0.00388 m2/s/10-6 s)0.5/1022 /m3) = 2.49 x 10-16 A. #

Example 3.6: For the device in Example 3.5, compute the forward current at Va = + 0.7 V Solution: From Eqn.(3-25), IF = Is x exp(qVa/kT) = 2.49 x 10-16 x exp(0.7 V/0.0259 V) A = 1.36 x 10-4 A. #

a)

Other current contributions

Other than the diffusion currents (which occur outside the depletion region), there are also generation current and recombination current within the depletion region. Generation current is due to thermal generation of electrons and holes in the depletion region. The process is illustrated in Fig.3.16. It is important during reverse bias when the depletion layer width is substantially widened.

Assuming a thermal generation rate given by G and a generation lifetime g, one can express G = ni g. This leads to a generation current density Jgen given by:

45

45

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

Jgen = oW qG dW = qniW/g

(3-26)

The total reverse current density in the presence of generation is: JR = Js + Jgen = qDppn0/Lp + qDnnp0/Ln. + qniW/g (3-27)

Recombination current exists primarily in the depletion region. A typical recombination process via an impurity center is shown in Fig.3.17. It differs from the generation process in the sense that it is important under forward bias.

Assuming a carrier recombination rate given by U = ((pn) ni2)/nir, where (pn) is the excess of the product of p and n, one can write: U = ni [exp(qVa/kT) - 1]/r (3-28)

where r = [nn + pn + 2ni cosh(Ei - Et)]/(ni 0vthNt), Et is the energy of the recombination center, Nt is the density of the recombination center, vth is thermal velocity, and 0 is the capture cross-section of the recombination center. Note that we have assumed the carrier capture cross-sections for the electron and the hole are the same and are equal to o.

46

46

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 47 -1/15/02C:\lec320.doc

H.L.Kwok

Theoretically, it can also be shown that the most effective recombination center is located when E t = Ei. This statement together with the assumption p n = nn = ni exp(qVa/2kT) (a situation chosen for maximum recombination probability) gives: Umax 0vthNt ni exp(qVa/2kT)/2 where we have assumed Va > 3kT/q. (3-29)

The recombination current density Jr is: Jr = q0W Umax dW = q Umax W (3-30)

The total forward current density now becomes: JF = Js exp(qVa/kT) + qW0vthNt ni exp(qVa/2kT)/2 (3-31)

In general, JF is proportional to exp(qVa/kT), where the ideality factor varies between 1 to 2. This is illustrated in Fig.3.18.

Within the P-N junction, high-injection results in current flow different from the normal currents. During high-injection, we have pn = nn = ni exp(qVa/2kT) and the total current density JT is given by: JT = Jo [exp(qVa/2kT) - 1] (3-32)

47

47

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

Thus, the current density increases at a slower rate with increasing bias voltage at high-injection. A typical plot showing high-injection in a P-N junction is given in Fig.3.19.

Example 3.7: For an ideal P-N junction with NA = 1023 /m3 and ND = 1021 /m3. Assume that it contains 1021 /m3 generation and recombination centers located 0.02 eV above the intrinsic Fermi level with n = p = 10-19 m2. For vth = 1 x 105 m/s, calculate the generation current at V a = - 0.5 V. Acs = 10-8 m2, g = 0.27 s, and p = 0.1 s. Solution: From Eqn.(3-5), Vbi = kT/q x ln(NAND/ni2) = 0.0259 V x ln(1023 /m3 x 1021 /m3/2.1 x 1032 /m6) = 0.695 V. From Eqn.(3-13), W = (2s(Vbi + VR)/(qND))0.5 = (2 x 11.9 x 8.86 x 10-12 F/m x (0.695 + 0.5) V/(1.6 x 10 -19 C x 1021 /m3))0.5 = 1.25 x 10-6 m. From Eqn.(3-26), Igen = Jgen x Acs = q niWAcs/g = 1.6 x 10-19 C x 1.45 x 1016 /m3 x 1.25 x 10-6 m x 10-8 m2/0.27 x 10-6 s = 1.1 x 10-10 A. #

Example 3.8: With Example 3.7, repeat the calculations for the recombination current when Va = 0.5 V. Assume r (= 0vthNt/2) = 0.1 s. Solution: From Eqn.(3-13), W = (2s(Vbi - Va)/(qND))0.5 = (2 x 11.9 x 8.86 x 10-12 F/m x (0.695 V - 0.5 V)/(1.6 x 10 -19 C x 1021 /m3))0.5 = 0.5 x 10-6 m. From Eqns.(29) and (30), Irec = qW niAcs exp(qVa/2kT)/g = 1.6 x 10-19 C x 0.5 x 10-6 m x 1.45 x 1016 /m3 x 10-8 m2 x exp(0.5 V/(2 x 0.0259 V))/0.1 x 10-6 s = 1.6 x 10-6 A. #

48

48

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 49 -1/15/02C:\lec320.doc

H.L.Kwok

b)

Charge storage

Under forward bias, minority carriers are stored in the P-N junction. Such charges will give rise to diffusion capacitance.

In a forward bias P-N junction, the hole charge per unit area stored in the N-region is given by: Qp = qxn (pn - pn0) dx = qxn pn0 (exp(qVa/kT) - 1) exp(- (x - xn)/Lp) dx = qLp pn0 (exp(qVa/kT) - 1) (3-33)

Since Jp = qDp pno/Lp [exp(qVa/kT) - 1], one can write: Qp = Lp2Jp/Dp = pJp This is illustrated in Fig.3.20. (3-34)

Similarly, Qn = nJn. Thus, QT(= Qp + Qn) = pJp + nJn. If p = n, QT JT. (3-35)

49

49

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

The diffusion capacitance per unit area C d is given by: Cd = Qp/Va = q2 Lp pn0/kT exp(qVa/kT) (3-36)

Note that diffusion capacitance increases with increasing forward bias. This is illustrated in Fig.3.21.

Fig.3.22 shows the equivalent circuit of a P-N junction including the capacitances.

d) Junction breakdown Breakdown occurs when there is excess current flowing through the P-N junction. Normally, breakdown is reversible provided there is a large external resistance that limits the current.

In a P-N junction, breakdown is normally either due to tunneling or avalanche multiplication. These processes are shown in Figs.3.23 and 3.24. Tunneling occurs in heavily doped P-N junctions. At reverse bias, tunneling occurs when the filled states in the P-side is right opposite to the unfilled states in the N-side so that electrons can

50

50

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 51 -1/15/02C:\lec320.doc

H.L.Kwok

tunnel through without energy change. This can result in a large current.

Avalanche multiplication is due to impact ionization of the carriers. Under a strong reverse bias, the electrons and holes gain enough energy before suffering a collision and upon impact with an atom, additional electrons and holes will be generated. Such a multiplication process is called avalanche multiplication.

Fig. 3.25 shows the (carrier) ionization rates during breakdown under different field intensities.

To estimate the breakdown voltage, one needs to define a critical field Ec. The breakdown voltage VB is: VB = ECW/2 (3-37)

Assuming EC = Em = qNBW/s in the case of a 1-sided step junction, one gets: VB = EC2 s/(2qNB) where NB is the substrate dopant density. (3-38)

Note that the breakdown voltage is inversely proportional to the substrate dopant density.5151

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

Fig.3.26 shows a plot of critical electric field versus the substrate dopant density.

Example 3.9: For a 1-sided step junction, what is the critical breakdown voltage when tunneling becomes important? Solution: From Fig.3.26, tunneling becomes important when EC = 8 x 107 V/m for NB = 5 x 1023 /m3. This leads to (from Eqn.(3.28)): VB = = EC2 s/(2qNB) = (8 x 107 V/m)2 x 11.9 X 8.86 X 10-12 F/m /(2 x 1.6 X 10-19 Coulomb X 5 X 1023 /m3 ) V = 4.21 V. #

52

52

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 53 -1/15/02C:\lec320.doc

H.L.Kwok

Part 4: Bipolar transistor

What we need to learn. Current components in a bipolar transistor a. Gain parameters b. Modes of operation c. Frequency characteristics d. Switching characteristics

53

53

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

Part 4: Bipolar transistor The word transistor refers to a transfer-resistance device.

This implies that the terminal resistances at the input and the output of the transistor are different. Structurally, a bipolar transistor is made up of 2 back-to-back P-N junctions. It is therefore possible to have either a NPN or a PNP transistor.

For simplicity we shall examine a 1-dimensional PNP transistor. This will be a 3 terminal device as shown in Fig.4.1. We label the terminals as emitter, base and collector. The dopant densities in each of the 3 regions will be different.

The operation of the transistor depends on the voltage bias (which characterizes the different modes of operation): For normal active operation, the emitter-base is forward biased and the collector base reverse biased. Its band diagram is shown in Fig.4.2. Note that the splitting of the Fermi-levels is indicative of the different biases.

A.

Current components in the active transistor

The following occurs during the formation of the PNP transistor:5454

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 55 -1/15/02C:\lec320.doc

H.L.Kwok

Hole current flowing from the emitter into the base

A portion of this current reaches the base-collector junction and they are labeled as IEp and ICp. Recombination of the holes occurs in the base

Electrons flow from the collector into the base due to the reverse bias and electrons flow into the emitter from the base due to the forward bias The currents are labeled as ICn, IEn and they are shown in Fig.4.3.

The total emitter current IE is given by: IE = IEp + IEn The total collector current IC is given by: IC = ICp + ICn (4-2) (4-1)

Since the transistor is a 3 terminal device, the base current I B is: IB = IE - IC = IEp + IEn - ICp - ICn These are illustrated in Fig.4.4. (4-3)

The efficiency of a PNP transistor is determined by the amount of hole current reaching the collector. This is expressed in terms of the common-base current gain 0 given by.5555

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

0 = ICp/IE = ICp/(IEp + IEn) = IEp/(IEp + IEn) x ICp/IEp (4-4)

The first term appearing in Eqn.(4-4) is the emitter efficiency . and the second term is the transport factor T. We can write: o = T. Furthermore, one has: IC = 0IE + ICn (4-5)

The collector current in the active mode consists of: a fraction of the emitter current

generation and diffusion currents in the reverse bias base collector junction

Since 0 is always less than 1 and I Cn is small, IC < IE.

a) Small-signal characteristics

The small signal characteristics are obtained under the following assumptions: dopant densities are uniform5656

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 57 -1/15/02C:\lec320.doc

H.L.Kwok

low-injection

absence of generation and recombination currents in the depletion regions absence of series resistance

Due to current injection from the emitter, the 1-dimensional hole (minority carrier) density in the base is given by: Dp d2pn/dx2 - (pn - pn0)/p = 0 (4-6)

This equation is subject to the following boundary conditions: pn(0) = pn0 exp(qVEB/kT) pn(WB) = 0 (4-7)

where x = 0 is at the edge of the emitter-base depletion region in the base, and WB is the base width.

The general solution is: pn = pn0 (exp(qVEB/kT) - 1) sinh((WB - x)/Lp)/sinh(WB/Lp) + pn0 (1 - sinh(x/Lp)/sinh(WB/Lp)) (4-8)

where we have made use of the relationship: L p2 = Dpp. Eqn.(4-8) gives the excess minority carrier distribution in the base which is shown in Fig.4.5. Note that sinh(z) = (exp(z) - exp(-z))/2.

57

57

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

For most P-N junctions, W B < Lp and we have: pn = pn0 (exp(qVEB/kT) - 1) (1 - x/WB) (4-9)

This is the excess minority carrier density distribution in the base.

The excess minority carriers stored in the base Q B is given by: QB = qAcsWB pn0 [exp(qVEB/kT) - 1]/2 where Acs is the area cross-section of the base. In a similar manner, we can obtain the minority carrier density distributions in the emitter and the collector. These are shown in Fig.4.6. (4-10)

Their values are: nE = nEo + nE0 (exp(qVEB/kT) - 1) exp((x + xE)/LE) nC = nC0 - nC0 exp(- (x - xC)/LC) x > xC x , - xE (4-11)

where nE is the electron density in the emitter, n E0 is the equilibrium value of nE, - xE is the edge of the depletion region in the emitter side, LE is the diffusion length for the electrons in the emitter, nC is the electron density in the collector, n C0 is the equilibrium value of nC, WB + xC is the edge of the depletion region in the collector side, and L C is the diffusion length for the electrons in the collector.5858

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 59 -1/15/02C:\lec320.doc

H.L.Kwok

Note that x is negative in the emitter.

We can now compute the diffusion currents in the different region: IEp = Acs [- qDp dpn/dx]x=0 = (qAcsDppn0/Lp) coth(WB/Lp) [(exp(qVEB/kT) - 1) + 1/cosh(WB/Lp)] (4-12)

where we have the relationship: cosh(z) = (exp(z) + exp(-z))/2 and coth(z) = cosh(z)/sinh(z).

For WB < Lp, IEp (qAcs Dp pn0/WB)(exp(qVEB/kT) - 1) + qAcsDpni2/(NBWB) (4-13) Similarly, at x = WB, ICp = qAcs Dp pn0/{Lpsinh(WB/Lp)} [(exp(qVEB/kT) - 1) + cosh(WB/Lp)] (qAcs Dp pn0/WB) [exp(qVEB/kT) 1] Thus, IEp ICp. (4-14)

For the electron current (assuming DE = DC = Dn),

59

59

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

IEn = Acs [- qDE dnE/dx]x = - xE = qAcs DEnE0 (exp(qVEB/kT) - 1)/LE ICn = Acs [- qDC dnC/dx]x = - xc = qAcs DCnC0/LC (4-15)

where DE is the electron diffusivity in the emitter, and D C is the electron diffusivity in the collector. We can write: IE = a11 (exp(qVEB/kT) - 1) + a12 (4-16)

When WB < Lp, we have: a11 = qAcs [Dpni2/(NBWB) + DEnE0/LE] a21 = qAcs Dpni2/(NBWB) where NB is the dopant density in the base. (4-17)

Note that IE = a12 when VEB = 0. This will be the diffusion current in the base when p n(0) = pn0 and pn(WB) = 0.

Similarly, we can write: IC = a21(exp(qVEB/kT) - 1) + a22 .6060

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 61 -1/15/02C:\lec320.doc

H.L.Kwok

For wB > Lp, a21 = qAcs Dpni2/(NBWB) a22 = qAcs [Dpni2/(NBWB) + DCnC0/LC] In addition, IB = IE - IC (4-19) (4-18)

Since QB = qAcsWB pn0 (exp(qVEB/kT) - 1)/2, it can be shown that both IE and IC are proportional to QB, the base charge.

It should be pointed out that the base current actually arises from carrier recombination as the carriers transit through the base.

From Eqn.(4-6): Dp d2pn/dx2 - (pn - pn0)/p = 0, Jp = - qDpdpn/dx = constant if recombination is absent. The base current is therefore suppressed when p is large.

Finally, we can evaluate the emitter efficiency and the transport factor. They are given as: = IEp/(IEp + IEn) = 1/(1 + IEn/IEp) 1/[1 + (qAcsDEnE0/LE) (exp(qVEB/kT) - 1)/{(qAcs Dppn0/WB)6161

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

(exp(qVEB/kT) 1)}] 1/(1 + DEnE0WB/(Dppn0LE)) (4-20)

Thus, T = ICp/IEp {qAcsDppn0(exp(qVEB/kT) 1)/(Lp sinh(WB/Lp)}/[(qAcs Dppn0/WB) (exp(qVEB/kT) - 1)] 1 - WB2/(2Lp2) (4-21)

For an efficient device, it is desirable to have both and T close to 1

Example 4.1: A silicon P+-N-P transistor has impurity densities of 5 x 1024 /m3, 1022 /m3 and 1021 /m3 in the emitter, base and collector, respectively. The base width is 1 m and the device cross-section is 3 mm x 3 mm. When the emitter-base junction is forward-biased to + 0.5 V and the basecollector junction is reverse-biased to - 5 V, calculate the neutral base width (physical base width minus the depletion layer widths). Solution: From Eqn.(3-5): Vbi = kT/q x ln(NCNV/ni2) = 0.0259 V x ln(1022 /m3 x 1021 /m3/2.1 x 1026 /m3) = 0.636 V. The depletion layer width in the base-collector junction = (2s(Nbase + Ncollector)(Vbi + VCB)/(qNbaseNcollector))0.5 = (2 x 11.9 x 8.86 x 10-12 F/m x (10226262

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 63 -1/15/02C:\lec320.doc

H.L.Kwok

/m3 + 1021 /m3 x (0.636 V + V)/(1.6 x10-19 C x 1022 /m3 x 1021 /m3))0.5 = 2.85 m. The depletion region on the collector side that extends into the base = WBC/(1 + Nbase/Ncollector) = 2.85 m/(1 + 1022 /m3/1021 /m3) = 0.26 m. A similar calculation for the emitter-base junction gives a depletion region in the base of 0.217 m. The neutral base width = (1 - 0.26 -0.217) m = 0.523 m. #

Example 4.2: For the transistor in Example 4.1, assume that the diffusivities of the minority carriers are 0.0002, 0.001 and 0.0035 m 2/s and the corresponding lifetimes are 0.01, 0.1 and 1 s, respectively, determine the current components: I Ep, ICp and IB. Solution: It can be shown that: L En = 1.41 m, LBp = 10 m and LCn = 59.2 m. From Eqn.(4-12): IEp = qAcsDppn0/Lp coth(WB/Lp) [(exp(qVEB/kT) - 1) + 1/cosh(WB/Lp)] = 1.6 x 10-19 C x (3 x 10-3 m)2 x 0.0002 m2/s x 2.1 x 1026 /m6/1022 /m3 x coth(0.523 m/10 m) x (exp(0.5 V/0.0259 V) - 1) + 1/(cosh(0.523 m/10 m)) = 4.6714 mA. # Similarly, it can be shown that (based on Eqn.(4-13)): I Cp = 4.6650 mA. # IB = IEp - ICp = 6.38 A. #

Example 4.3: If NA in the emitter is 1025 /m3, ND in the base is 1023 /m3 and NA in the collector is 5 x 10 21 /m3, compute 0 for DE = 10-4 m2/V.s, Dp = 103 m2/V.s, LE = 1o-6 m, Lp = 10-5 m, and WB = 0.5 x 10-6 m.

63

63

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

Solution: From Eqn.(4-20): 1/(1 + DEnE0WB/(Dppn0LE)) = 1/(1 + 10-4 m2/s x 1023 /m3 x 0.5 x 10-6 m /(10-3 m2/s x 1025 /m3 x 10-6 m)) = 0.9995. T 1 2 2 WB /(2Lp ) = 0.9987. Therefore, 0 = T = 0.9982. #

B.

Modes of operation

The following are the different modes of operation for the bipolar transistor: bias Active mode - VEB is at forward bias while VBC is at reverse

Saturation mode - VEB is at forward bias while VBC is also at forward bias Cutoff mode - VEB is at reverse bias while V BC is also at reverse bias Inverted mode - VEB is at reverse bias while V BC is at forward bias

Fig. 4.7 shows the output characteristics of a typical bipolar transistor showing the active region, saturation and cutoff. Active mode corresponds to the case when the output behaves as a current source dependent on the value of the input voltage.

64

64

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 65 -1/15/02C:\lec320.doc

H.L.Kwok

Saturation occurs when both the input junction and output P-N junction are at forward bias and there is very little resistance across the terminals of the transistor. Cutoff implies that little or no current is allowed to pass through the terminals.

D.

Equivalent circuit models for the bipolar transistor

Eber-Moll model - This model is constructed using 2 back-to-back P-N junctions as shown in Fig.4.14. The governing equations are: IE = IF0 (exp(qVEB/kT) - 1) - RIR0 (exp(qVCB/kT) - 1) IC = F IF0(exp(qVEB/kT) - 1) - IR0 (exp(qVCB/kT) - 1) (4-24)

where IF0 is the forward saturation current of the emitter-base junction, IR0 is the reverse saturation current of the basecollector junction, F is the forward common-base current gain, and R is the reverse common-base current gain. The above equations can apply to the different modes of operation including the use of large signals.

E. Frequency response of the bipolar transistor The response of the bipolar transistor can be separated into the dc and ac components.

65

65

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

The frequency response is usually included in the small-signal analysis. In general, the currents and the terminal voltages can be expressed as (Total = dc + ac (small signal)): i E = I E + i E vEB = VEB + vEB i C = IC + i C vCB = VCB + vCB i B = I B + i B (4-25)

where iE, iB and iC are the total currents, IE, IB and IC are the dc components, and iE, iB and iC are the ac components.

The subscripts E, B and C stand for the emitter, base and collector, respectively. Similar notations apply to the voltages.

For the active mode of operation, we have: iE = IFo exp(qVEB/kT) iC = F IFo exp(qVEB/kT) iB = (1 - F )IFo exp(qVEB/kT) (4-26)

Thus, for a small change in the emitter-base voltage v EB, we have: iC = IC + d(iC)/dVEB|VEC vEB = IC + iC6666

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 67 -1/15/02C:\lec320.doc

H.L.Kwok

iB = IB + d(iB)/dVEB|VEC vEB = IB + iB

(4-27)

This leads to: iC = gmvEB and iB = gEBvEB, where gm is the transconductance, and gEB is the conductance of the emitter-base junction.

In addition, gm = d(iC)/dVEB|VEC = (q F IF0/kT) exp(qVEB/kT) = F qIE/kT gEB = d(iB)/dVEB|VEC = q (1 - F) IE/kT = qIB/kT (4-28)

From Eqn.(4-27), iC, iB and vEB form the small-signal ac parameters of the device. Fig.4.15 shows the small-signal equivalent circuit for the bipolar transistor.

The frequency response of the bipolar transistor can be linked to the gain parameters as shown in Fig.4.16.

In general, the frequency-dependent common-base current gain is given by: = 0/(1 + jf/f) (4-29)

where 0 is the low frequency common-base current gain, and f is the common-base cutoff frequency.

67

67

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

Similarly, the frequency-dependent common-emitter current gain is given by: = 0/(1 + jf/f) where f is the common-emitter cutoff frequency. (4-30)

Since = /(1 - ), we have: f = (1 - 0)f and f < f . (4-31)

Both f and f are called the 3-dB frequencies meaning that at these frequencies, and both reduce to 0.707 of their initial values. Note that the 3 dB frequency points are the half-power points.

The unity-gain cutoff frequency fT is often quoted in the specifications of transistors. It occurs when = 1. Thus, = 0/(1 + jfT/f)) = 1 fT = f (02 - 1) 0 f 0f This implies: fT f. (4-32)

68

68

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 69 -1/15/02C:\lec320.doc

H.L.Kwok

The ultimate frequency limit for the operation of the bipolar transistor is given by the inverse of the time required for an injected carrier to cross the base as illustrated in Fig.4.17. This is called the transit time B. Transit time is given by: B = oWB (1/v).dx = oWB (qpnAcs/Ip).dx (4-33)

By setting pn = pn0 (1 - x/WB) and Ip = qAcsDppn0/WB, we have: B = 0WB [WB(1 - x/WB)/Dp].dx = WB2/(2Dp) (4-34)

The base width theoretically limits the frequency response of the bipolar transistor and fmax ~ 1/B.

F. Switching transients in the bipolar transistor In digital circuits, transistors are often required to switch from active to cutoff. The switching response depends on the charge storage in the base region. The simplest way to model the switching bipolar transistor is to assume the existence of an OFFresistance Roff and an ON-resistance Ron. The circuit schematic is shown in Fig.4-18.

These resistances are given by: Roff = VC/IC(off)

69

69

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

Ron = VCE(on)/IC

(4-35)

The switching time is given by the time required to switch between these 2 states.

For a common-emitter transistor to switch from off to on, the base charge simply builds up from cutoff to saturation as shown in Fig.4-19.

The base charge QB is given by: QB = qAcs 0WB (pn - pn0) dx (4-36)

The time evolution of the base charge can be obtained in the following manner: dpn/dt = - 1/q dJp/dx - (pn - pn0)/p Integrating from x = 0 to x = WB gives: Ip(0) - Ip(WB) = dQB/dt + QB/p Since Ip(0) - Ip(WB) = iB, we have: dQB/dt + QB/p = iB QB = iBp (1 - exp(- t/p)) (4-39) (4-38) (4-37)

Thus, QB changes from 0 (OFF) to iBp (ON). This is reflected in the lowering of the base voltage as shown in Fig.4.20.7070

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 71 -1/15/02C:\lec320.doc

H.L.Kwok

Assuming that the bipolar transistor is saturated (this corresponds to the situation when the base-collector junction also becomes forward bias) at t = t1 and QB = Qsat, then Qsat = iBp (1 - exp(- t1 /p)) t1 = p ln(1/(1 - Qsat/IBp)) (4-40)

In general, Qsat = VCp/RL.

The turn-off transient should be the reverse of the turn-on transient. If t = t2 is the initial turn-off time, one gets: QB = QB(t2) exp(- (t - t2)/ p) (4-41)

Turn-off comes in 2 stages.

The first stage involves charge removal while the device remains in saturation and the second stage involves a progressive decrease in the output current. The time tsat in the first stage is the storage time. Since Qsat = QB(t2) exp(- (t3 - t2)/ p), where QB = Qsat when t = t3, we have: tsat = t3 - t2 = p ln((QB(t3)/Qsat)71

(4-42)71

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

The second stage involves the reduction in the charge gradient in the base and the collector current will decrease as: iC = (QB(t3)/ p) exp(- (t - t3)/ p) (4-43)

Example 4.7: A switching transistor has a base width of 0.5 m and a diffusivity of 0.001 m2/s. The minority carrier lifetime in the base is 0.1 s and VCC = 5 V and RL = 10 k. If the base current is a 1 s pulse at 2 A, find the stored charge in the base and the storage time delay. Solution: From Eqn.(4-39), the base charge QB = IBp (1 - exp(- t1 /p)) = 2 x 10-6 A x 10-7 s x (1 - exp(- 10-6 s/10-7 s)) = 2 x 10-13 C. # At saturation, Qsat = VCCB /RL = VCC (W2/2DB)/RL = 5 V x (5 x 10-7 m)2/(2 x 10-3 m2/s)/104 = 6.25 x 10-14 C. From Eqn.(4-42), the storage time tsat = p ln(QB(t2)/Qsat) = 10-7 s x ln(2 x 10-13 C/6.25 x 10-14 C) = 0.116 s. #

72

72

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 73 -1/15/02C:\lec320.doc

H.L.Kwok

Part 5: MIS diode and MOS transistor

What we need to learn. Physical properties of the MIS diode Capacitance characteristics Physical structure of the MOS transistor I-V characteristics Other effects urrent components in a bipolar transistor a. Gain parameters b. Modes of operation c. Frequency characteristics d. Switching characteristics

73

73

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

Part 5:

MIS diode and MOS transistor

The electrical properties of the MOS transistor are primarily determined by the properties of the MIS diode. We first consider the ideal MIS diode and its characteristics:

A.

MIS diode

The MIS diode is a two terminal device similar to a PN junction although structurally it is no different from a capacitor Since there is no dc current passing through a capacitor, the parameter of interest is its capacitance, which varies with the applied voltage.

a) Potential distribution in the MIS diode The MIS diode is in a way similar to the reverse bias P-N junction. Structurally, it consists of a metal gate, an oxide layer, and a substrate semiconductor, which we assume to be P-type. This is illustrated in Fig.5.1. Because of the different possible combination of MIS structures and the presence of non-idealities, we shall begin with the ideal initial condition that all of the energy bands are flat, i.e., qms = qm - [q + Eg/2 + qB] = 0 (5-1)

74

74

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 75 -1/15/02C:\lec320.doc

H.L.Kwok

where m is the metal work function, is the electron affinity, and B is the energy difference between the Fermi-level and the intrinsic Fermi-level. The above is the flat-band condition and it assumes the absence of space charge in the oxide. Fig.5.2 shows the energy band diagram for the MIS diode under flat-band condition.

When a voltage is applied across the MIS diode, the following may result: When VG is small and positive, the substrate will be depleted; i.e., holes will be withdrawn from the interface and the acceptors are exposed When VG is large and positive, the substrate will be inverted near the interface but further into the substrate, there is a depletion region When VG is negative, holes will be attracted to the oxidesemiconductor interface and a hole accumulation layer will exist These are known as depletion, inversion, and accumulation, respectively. The conditions are shown in Fig.5.3.

75

75

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

Similar to a parallel-plate capacitor, charge conservation is observed in the MIS diode and we have: QS = Qn + QSC = - Qm (5-2)

where QS is the semiconductor charge per unit area, Qn is the inverted charge per unit area, QSC is the depletion layer charge per unit area, and Qm is the electrode charge per unit area. These charge layers are shown in Fig.5.4. In the absence of Qn, the depletion charge density QSC = - qNAW, where W is the depletion layer width.

Inside the MIS diode, the charge states in the semiconductor are best described by their potential denoted by . Since the energy bands are drawn for electrons, positive potential (and ) will increase downward. The value of right at the oxide-semiconductor interface is the surface potential, s. With this notation, inversion occurs when s > B; depletion occurs when B > s > 0; and accumulation occurs when s < 0. B is the energy difference between the Fermi-level and the intrinsic Fermi-level.

76

76

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 77 -1/15/02C:\lec320.doc

H.L.Kwok

Note that is zero in the bulk and this is shown in Fig.5.4.

The carrier densities in the P-type semiconductor can be written as: pp = ni exp((Ei - EF)/kT) np = ni exp(- (Ei - EF)/kT) (5.3)

For the P-type substrate, we have Ei = - q and EF = - qB. This leads to: pp = ni exp(q(B - )/kT) np = ni exp(- q(B - )/kT) (5-4)

We can now use the above equations to determine the carrier densities. At the oxide-semiconductor interface, we have = s. If s < B, pp > ni, we have either depletion or accumulation. On the other hand, if s > B, pp < ni, and we have inversion.

The electrostatic potential in the semiconductor can be computed using Poisson equation, i.e.,7777

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

d2/dx2 = - /s = qNA/s

(5-5)

Assuming a depletion layer width W and boundary conditions such that = o and d/dx = 0 at x = W, we have: = s (1 - x/W)2 where s = qNAW2/(2s). Thus, the surface potential changes as W 2. (5-6)

Normally, surface inversion is fully formed when s = 2B. This corresponds to the situation when the surface electron density n| x = 0 NA. This is known as strong inversion.

Once the inversion layer is fully formed, the depletion layer width reaches its maximum value and it is given by: Wm = (2sB/(qNA))

(5-7)

Similarly,

78

78

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 79 -1/15/02C:\lec320.doc

H.L.Kwok

QSC = - qNAWm

(5-8)

Example 5.1: For an ideal Si-SiO2 MIS diode with d = 30 nm and NA = 5 x 1021 /m3, find the applied voltage required to make the silicon surface: i) intrinsic; and ii) in strong inversion. Solution: The oxide capacitance C0 = 3.9 x 8.86 x 10-12 F/m/3 x 10-8 m = 1.15 x 10-3 F/m2. i) For the Si surface to be intrinsic: = B = kT/q x ln(NA/ni) = 0.0259 V x ln(5 x 1021 /m3/1.56 x 1016 /m3) = 0.33 V. Ideal diode implies VFB = 0 and Va = B + (2 sqNAB)0.5/Co = 0.33 V + (2 x 11.9 x 8.86 x 10-12 F/m x 1.6 x 10-19 C x 5 x 1021 /m3 x 0.33 V)0.5/1.15 x 10-3 F/m3 = 0.53 V. # ii) For strong inversion: = 2B. This leads to: V a = 0.95 V. #

b) C-V characteristics of the MIS diode In the presence of an applied bias, the voltage drop across the MIS diode can be expressed as: Va = V0 + s (5-9)

where V0 is the voltage drop across the oxide and s is the surface potential.

79

79

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

In general, we see that the applied voltage is dropped across two different regions. One region is the oxide layer and there we have: V0= Qsd/ox, where d/ox = 1/C0, and C0 is the oxide capacitance per unit area. Another component of Va is dropped across the space charge region, and the associated capacitance per unit area C SC is given by: CSC = s /W = (qsNA/(2s)) = [qsNA/(2(Va - V0 ))] (5-10)

At strong inversion, Qs = qNAWm. This leads to: Va = qNAWm/C0 + 2B This is the threshold voltage VT for the MIS diode. (5-11)

Fig.5.5 shows the C-V characteristics of the MIS diode under different bias conditions and at different frequencies.

c) Flat-band voltage

80

80

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 81 -1/15/02C:\lec320.doc

H.L.Kwok

The flat-band condition mentioned earlier is rarely observed in nature and in general qms is not zero. Flat-band condition can be achieved by introducing a parameter called flat-band voltage VFB. In general, the flat-band voltage is given by: VFB = ms + (Qf + Qm + Qot + Qit)/C0 (5-12)

where ms is the metal-semiconductor work function, Q f is the oxide fixed charge density, Qm is the oxide mobile charge density, Qot is the oxide trap charge density, and Qit is the interface trap charge density.

Example 5.2: For a Si-SiO2 MIS diode at 300 K with d = 30 nm, NA = 5 x 1021 /m3; the metal work function is 3 eV, q = 4.05 eV, Qf/q = 1015 /m2, Qm/q = 1014 /m2, Qot/q = 5 x 1014 /m2 and Qit = 0, determine the flat band voltage. Solution: As shown in Example 5.1: C0 = 1.15 x 10-3 F/m2. From Eqn.(5-12), VFB = ms + (Qf + Qm + Qot + Qit)/C0 = 3 V - 4.05 V + 1.6 x 10-19 C(1015 C + 1014 C + 5 x 1014 C)/(1.15 x 10-3 F/m2) = - 1.27 V. #

81

81

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

B.

MOS transistor

MOS transistor is also called MOSFET (metal-oxidesemiconductor field-effect transistor) The device consists of a MIS diode with two PN junctions on either side. A schematic of a MOSFET is shown in Fig.5.6. The input to the device is the gate (the top electrode of the MOS diode) and the output is the current passing (laterally) through the PN junctions. The output terminals are called the drain and the source (the source is the source of electrons, i.e., the terminal where current leaves).

In the following, we shall examine the I-V characteristics of an Nchannel device, i.e., the substrate semiconductor is P-type. A schematic of such a device is shown in Fig.5.7. For any appreciate current to pass through the device, an inversion layer or channel underneath the gate must exist. This normally requires a positive gate voltage exceeding the threshold voltage of the MIS. In addition, we assume that the source and the substrate are grounded and a positive voltage is applied to the drain.

82

82

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 83 -1/15/02C:\lec320.doc

H.L.Kwok

a) I-V characteristics of the MOS transistor The I-V characteristics of the MOS transistor is derived with the following ideal conditions (see Fig.5.7): flat-band condition only drift currents are important carrier mobilities are constant doping in the channel is uniform reverse leakage currents are small

transverse electric field in the channel is much smaller than the longitudinal electric field

Semiconductor charge present in the MOS transistor can be expressed as: Qs = Qn + QSC (5-13)

where Qs is the semiconductor charge density; Q n is the electron density in the channel, and QSC is the space charge density present in the depletion region. Since Qs = - (VG -s )C0 and QSC = - (2sqNA (Va + 2B)), one gets:

83

83

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

Qn = C0 (VG - Va - 2B ) + (2sqNA (Va + 2B))

(5-14)

This equation gives the electron density in the inversion layer per unit area.

The resistance associated with this inversion layer can be written as: R= y/(ZnQn) (5-15)

where Z is the width of the device, n is the electron mobility, and y is incremental distance in the direction of current flow.

Since V = IDR, and ID is the current in the inversion layer, one gets: 0L ID.dy = 0VD Zn Qn.dV (5-16)

where L is the channel length, and VD is the drain voltage.

Combining Eqn.(5-14) and (5-16) leads to: ID = Zn(C0/L) [(VG - 2B - VD/2) VD {(8sqNA)/3C0} .((VD + 2B)3/2 - (2B)3/2)] (5-17) This equation gives the I-V characteristics of the MOS transistor.8484

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 85 -1/15/02C:\lec320.doc

H.L.Kwok

A graphical plot is shown in Fig.5.8.

The I-V characteristics of the MOS transistor can be subdivided into the linear region and the saturation region. In the linear region, VD is small and we can write: ID Zn (C0/L) (VG - VT) VD where VT = (4sqNAB)/C0 + 2B. Thus, ID is proportional to VD and we can define a channel conductance gD given by: gD = Zn (Co/L) (VG - VT) (5-19) (5-18)

Saturation occurs when the channel pinches off and this happens when Qn = 0 as y = L. Eqn.(5-14) now has the form: x2 + (2)K2 x - VG = 0, where x = (Va + 2B) and K2 = (sqNA)/C0. Solving this leads to: x = [- (2) K2 +/- (2K22 + 4 VG)]/2. By setting Va = VDsat, one gets:

85

85

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

VDsat = VG - 2B + K2 [1 - (1 + 2VG/K2)1/2]

(5-20)

If we substitute Vdsat into the I-V characteristics of the MOSFET, this leads to: IDsat Znox (VG - VT)2/(2dL) where d is the oxide thickness. (5-21)

In addition, we define transconductance gm given by: gm = Zn ox(VG - VT)/(dL) (5-22)

Fig.5.9 shows the equivalent circuit for the MOSFET in saturation.

Example 5.3: Consider a long channel MOSFET with L = 3 m, Z = 21 m, NA = 5 x 1021 /m3, C0 = 1.5 x 10-3 F/m2 and VT = 1.5 V. Determine VDsat when VG = 4 V. Solution: The substrate potential B = kT/q x ln(NA/ni) = 0.0259 V x ln(5 x 1021 /m3/1.56 x 1016 /m3) = 0.33 V. K = (sqNA)/C0 = (11.9 x 8.86 x 10-12 F/m x 1.6 x 10-19 C x 5 x 1021 /m3)0.5/1.5 x 10-3 F/m2 = 1.93 x 10-2 V0.5.

86

86

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 87 -1/15/02C:\lec320.doc

H.L.Kwok

From Eqn.(5-20), VDsat = VG - 2B + K2[1 - (1 + 2VG/K2)0.5] = 4 V - 2 x 0.33 V + 3.72 x 10-4 V x (1 - (1 + 2 x 4 V/3.72 x 10 -4 V)0.5) = 3.40 V. #

b) Frequency response When the output of the MOS transistor is short-circuited, the input current is given by: iin = j(CGS + CGD) vG jC0ZLvG. where vG is the ac gate voltage. (5-23)

Since the output current is iout = gmvG, unity gain occurs when C0ZL = gm.

The cutoff frequency is given by: fT = /2 = gm/(2 C0ZL) = nVD/(2 L2) (5-24)

Note that fT is inversely proportional to L2 and we have used the relationship VD = VG - VT.

c) Subthreshold conduction

87

87

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

Below threshold, the MOS channel is not fully formed and a horizontal PNP transistor is present as shown in Fig.5.10. The lateral current will be primarily due to diffusion and it is given by: ID = - qAcsDn dn/dy = qAcsDn (n(0) - n(L))/L (5-25)

Since n(0) = nI exp(q(s - B)/kT), and n(L) = nI exp(q(s - B VD)/kT), it can be shown that: ID = qAcsDn ni exp(- qB/kT) [1 - exp(- qVD/kT)] exp(qs/kT)/L (5-26) Since s = VG - VT, we have for a small VD: ID exp(- q(VG - VT)/kT) (5-27)

where VT is the threshold voltage of the MOS transistor.

The threshold current is exponentially proportional to the gate voltage. This is similar to the case of the bipolar junction transistor where the output collector current is proportional to the emitterbase voltage.

88

88

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 89 -1/15/02C:\lec320.doc

H.L.Kwok

d)

Enhancement mode and depletion mode devices

In addition to N-channel and P-channel MOS transistors, these devices can operate in the enhancement mode or the depletion mode. Enhancement mode transistors are normally OFF and a gate bias is required to form the channels (ON). The channel of a depletion mode device is formed in the absence of any bias.

e) Threshold voltage under non-ideal conditions Most MOS transistors do not exhibit flat-band condition in the absence of bias and a flat-band voltage is required to achieve flatband condition. In general, VT = VFB + 2B + (4sqNAB)/C0 (5-28)

Normally, in a P-channel device, a negative V T implies an enhancement mode device and a gate voltage more negative than VT is required to turn the device ON. For an N-channel device, a negative VT implies a depletion mode device and a gate voltage more positive than - V T is required to keep the device on.

Example 5.4: If the substrate dopant density of a MOS transistor is 10 20 /m3. Compute the threshold voltage if the substrate is: i) P-type; and ii) N-type. Assume an oxide thickness of 65 nm.8989

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

Solution: i) For a P-type substrate: qms = - 0.96 eV (see Fig.E5.1). B = kT/q ln(NA/ni) = 0.0259 x ln(1020/(1.45 x 1016) V = 0.229 V. Cox = ox/d = 3.9 x 8.86 x 10-12/(650 x 10-10) F/m2 = 5.3 x 10-4 F/m2. # VTN = VFB + 2B + (4sqNAB)/C0 = - 0.96 + 2 x 0.229 + (2 x 11.9 x 8.86 x 10-12 x 1020 x 0.458)/5.3 x 10-4 = - 0.42 V. # ii) For an N-type substrate, qms = - 0.51 eV. VTP = VFB + 2B + (4sqNDB)/C0 = - 0.52 - 2 x 0.229 - (2 x 11.9 x 8.86 x 10-12 x 1020 x 0.458)/5.3 x 10-4 = - 1.04 V. # Note that as B increases, VTN increases while VTP decreases.

f) Substrate bias A reverse bias in the substrate affects the space charge in the depletion layer. Substrate bias is normally applied at the source and this increases the depletion layer width such that: Wm = (2s (2B + VBS)/qNA) Similarly, VTN = VFB + 2B + [2sqNA (2B + VBS)] /C0 (5-29)

90

90

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 91 -1/15/02C:\lec320.doc

H.L.Kwok

VTN = (2sqNA/C0) [(2B + VBS)1/2 - (2B)1/2]

(5-30)

Substrate bias therefore increases the threshold voltage in a Nchannel device.

g) Device scaling Device scaling is intended to increase the device density per unit area while not affecting substantially the transistor characteristics

Disadvantages observed in scale-down device are: 2-dimensional and high-field effects often limit the device performance. High field effects tend to cause breakdown between the drain and the source. Mobility saturation can degrade the frequency performance. At very high electric field, velocity saturation occurs when v sat 1 x 105 m/s.

When vdrift = vsat, IDsat = Zqvsat 0xi n.dx, where xi is the thickness of the depletion layer.

91

91

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

Since Qn = 0xi n dx C0 (VG - VT), one gets: IDsat = ZC0 vsat (VG - VT) gm = ZC0vsat (5-31)

Compare this with normal operation (when gm = Z C0n (VG VT)/L), gm is reduced considerably.

For a scaling factor of k (k >1), we have: L = L/k, d = d/k, Z = Z/k, Va = Va/k (5-31)

This leads to: IDsat = (Z/k) kCovsat (VG - VT)/k = IDsat /k JDsat = JDsat k Pac = CoAcs Va2/(2RCoAcs) = Pac/k2

92

92

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

- 93 -1/15/02C:\lec320.doc

H.L.Kwok

Pdc = IVa = Pdc/k2 Note that in this case, only J Dsat is increased.

(5-32)

To avoid short-channel effect (such as velocity saturation and 2 dimensional effect), there is an empirical relationship for the minimum channel length. It is given by: Lmin = 0.4 [rjd(Ws + WD)2]1/2 (5-33)

where rj is the junction curvature, and W s and WD are the depletion layer widths in the source and the drain, respectively.

Example 5.6: Design a sub-micron MOSFET with a gate length of 0.75 m. (The gate length is the channel length plus twice the junction depth.) If the junction depth is 0.2 m, the gate oxide thickness is 20 nm, and the maximum drain voltage is limited to 2.5 V, find the required channel doping so that the MOSFET can maintain its long channel characteristics. Solution: The channel length L = 0.75 m - 2 x 0.2 m = 0.35 m. From Eqn.(5-33), Lmin = 0.4 [rjd(Ws + WD)2]1/3. If Lmin = L, Ws + WD = (0.35 m/0.4)3/(0.2 x 200) = 0.129 m. Since WD Ws + WD and VR VR + Vbi, NB (min) = (2 sVR/(qWD2)) = 2 x 11.9 x 8.86 x 10-12 F/m x 2.5 V/(1.6 x 10-19 C x 11.8 x (0.129 x 10-6 m)2) = 1.97 x 1023 /m3. #

93

93

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com

c:\book3.doc

END

94

94

PDF created with FinePrint pdfFactory trial version http://www.fineprint.com